Phase Diagrams

# Phase Diagrams

## Phase Diagrams

- - - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - - -
##### Presentation Transcript

1. Phase Diagrams Chapter 10

2. Chapter 10 (part 1) • Introduction • Solubility Limits • Phases • Phase Equilibrium • Interpretation of Phase Diagrams • Binary Isomorphous Systems (Cu-Ni) • Development of Microstructure • Mechanical Properties • Binary Eutectic Systems • Development of Eutectic Alloy Microstructure

3. Components and Phases • Components: The elements or compounds that are mixed initially (Al and Cu). • Phases: A phase is a homogenous, physically distinct and mechanically separable portion of the material with a given chemical composition and structure (a and b). Aluminum- Copper Alloy

4. Sugar/Water Phase Diagram 10 0 Solubility L Limit 8 0 (liquid) 6 0 + L Temperature (°C) S (liquid solution 4 0 i.e., syrup) (solid 20 sugar) 0 20 40 60 80 100 C = Composition (wt% sugar) Water Sugar Phase Equilibria: Solubility Limit • Solution – solid, liquid, or gas solutions, single phase • Mixture – more than one phase • Solubility Limit: Maximum concentration for which only a single phase solution exists. Question: What is the solubility limit for sugar in water at 20°C? Answer: 65 wt% sugar. At 20°C, if C < 65 wt% sugar: syrup At 20°C, if C > 65 wt% sugar: syrup + sugar 65

5. Equilibrium • A system is at equilibrium if its free energy is at a minimum, given a specified combination of temperature, pressure and composition. • The (macroscopic) characteristics of the system do not change with time — the system is stable. • A change in T, P or C for the system will result in an increase in the free energy and possible changes to another state whereby the free energy is lowered.

6. One Component Phase Diagram

7. T(°C) 1600 1500 L (liquid) 1400 a liquidus + 1300 L solidus a 1200 (FCC solid 1100 solution) 1000 wt% Ni 0 20 40 60 80 100 Phase Diagrams • Indicate phases as a function of Temp, Comp and Pressure. • Focus on: - binary systems: 2 components. - independent variables: T and C (P = 1 atm is almost always used). • 2 phases: L (liquid) a (FCC solid solution) • 3 different phase fields: Cu-Ni system L a L + a

8. Effect of Temperature & Composition (Co) T(°C) 1600 1500 L (liquid) 1400 liquidus a + 1300 L solidus a 1200 (FCC solid solution) 1100 1000 wt% Ni 0 20 40 60 80 100 • Changing T can change # of phases: path A to B. • Changing Co can change # of phases: path B to D. D B Cu-Ni system A Cu

9. Determination of phase(s) present • Rule 1: If we know T and Co, then we know: --how many phases and which phases are present. • Examples: Cu-Ni phase diagram Melting points: Cu = 1085°C, Ni = 1453 °C Solidus - Temperature where alloy is completely solid. Above this line, liquefaction begins. Liquidus - Temperature where alloy is completely liquid. Below this line, solidification begins.

10. Phase Diagrams: composition of phases At TA = 1320°C: Only Liquid (L) present CL = C0 ( = 35 wt% Ni) At TD = 1190°C: Only Solid (a) present C = C0 ( = 35 wt% Ni) At TB = 1250°C:  Both and L present CL = C ( = 32 wt% Ni) liquidus C = C ( = 43 wt% Ni) solidus • Rule 2: If we know T and Co, then we know: --the composition of each phase. Cu-Ni system • Examples:

11. Phase Diagrams: weight fractions of phases • Rule 3: If we know T and Co, then we know: --the amount of each phase (given in wt%). • Examples: Cu-Ni system = 27wt %

12. Ex: Equilibrium Cooling of a Cu-Ni Alloy L: 35 wt% Ni B a: 46 wt% Ni 35 46 C 32 43 D L: 32 wt% Ni 24 36 a: 43 wt% Ni E L: 24 wt% Ni a: 36 wt% Ni T(°C) L: 35wt%Ni L (liquid) • Phase diagram: Cu-Ni system. Cu-Ni system a 130 0 A + L • Consider microstuctural changes that accompany the cooling of a C0 = 35 wt% Ni alloy a + 120 0 L a (solid) 110 0 35 20 3 0 4 0 5 0 wt% Ni C0

13. c10f05 • Development of microstructure during the non-equilibrium solidification of a 35 wt% Ni-65 wt% Cu alloy outcome: • Segregation-nonuniform distribution of elements within grains. • Weaker grain boundaries if alloy is reheated.

14. Cored vs Equilibrium Phases • Cachanges as it solidifies. • Cu-Ni case: Firstato solidify has Ca= 46wt%Ni. Last ato solidify has Ca= 35wt%Ni. • Fast rate of cooling: Cored structure • Slow rate of cooling: Equilibrium structure • Coring can be eliminated by means of a homogenization heat treatment carried out at temperatures below the alloy’s solidus. During the process, atomic diffusion produces grains that are compositionally homogeneous.

15. Mechanical Properties:Cu-Ni System • Effect of solid solution strengthening on: --Tensile strength (TS) --Ductility (%EL,%AR) --Peak as a function of Co --Min. as a function of Co

16. Binary Isomorphous Systems Cu-Ni system: • The liquid L is a homogeneous liquid solution composed of Cu and Ni. • The αphase is a substitutional solid solution consisting of Cu and Ni atoms with an FCC crystal structure. • At temperatures below 1080 C, Cu and Ni are mutually soluble in each other in the solid state for all compositions. • The complete solubility is explained by their FCC structure, nearly identical atomic radii and electro-negativities, and similar valences. • The Cu-Ni system is termed isomorphous because of this complete liquid and solid solubility of the 2 components.

17. Criteria for Solid Solubility Simple system (e.g., Ni-Cu solution) • Both have the same crystal structure (FCC) and have similar electronegativities and atomic radii (W. Hume – Rothery rules) suggesting high mutual solubility. • Ni and Cu are totally soluble in one another for all proportions.

18. T(°C) 1600 1500 L (liquid) 1400 a liquidus + 1300 L solidus a 1200 (FCC solid 1100 solution) 1000 wt% Ni 0 20 40 60 80 100 Isomorphous Binary Phase Diagram • Phase diagram: Cu-Ni system. • System is: Cu-Ni phase diagram -- binary 2 components: Cu and Ni. -- isomorphous i.e., complete solubility of one component in another; a phase field extends from 0 to 100 wt% Ni.

19. Importance of Phase Diagrams • There is a strong correlation between microstructure and mechanical properties, and the development of alloy microstructure is related to the characteristics of its phase diagram. • Phase diagrams provide valuable information about melting, casting, crystallization and other phenomena.

20. Microstructure • In metal alloys, microstructure is characterized by the number of phases, their proportions, and the way they are arranged. • The microstructure depends on: • Alloying elements • Concentration • Heat treatment (temperature, time, rate of cooling)

21. Eutectic • A eutectic or eutectic mixture is a mixture of two or more phasesat a composition that has the lowest melting point. • It is where the phases simultaneously crystallize from molten solution. • The proper ratios of phases to obtain a eutectic is identified by the eutectic point on a binary phase diagram. • The term comes from the Greek 'eutektos', meaning 'easily melted.‘

22. The phase diagram displays a simple binary system composed of two components, A and B, which has a eutectic point. • The phase diagram plots relative concentrations of A and B along the X-axis, and temperature along the Y-axis. The eutectic point is the point where the liquid phase borders directly on the solid α + β phase; it represents the minimum melting temperature of any possible A Balloy. • The temperature that corresponds to this point is known as the eutectic temperature. • Not all binary system alloys have a eutectic point: those that form a solid solution at all concentrations, such as the gold-silver system, have no eutectic. An alloy system that has a eutectic is often referred to as a eutectic system, or eutectic alloy. • Solid products of a eutectic transformation can often be identified by their lamellar structure, as opposed to the dendritic structures commonly seen in non-eutectic solidification. The same conditions that force the material to form lamellae can instead form an amorphous solid if pushed to an extreme.

23. Binary-Eutectic Systems • Eutectic reaction L(CE) (CE) + (CE) cooling heating has a special composition with a min. melting T. 2 components T(°C) Cu-Ag system 1200 • 3 single phase regions L (liquid) (L, a, b) 1000 a L + a • Limited solubility: b L + 779°C b 800 TE a: mostly Cu 8.0 91.2 71.9 b: mostly Ag 600 • TE : No liquid below TE a + b 400 • CE : Composition at temperature TE 200 80 100 0 20 40 60 CE C , wt% Ag

24. c10f07 Copper-Silver Phase Diagram

25. Eutectic reaction L(CE) (CE) + (CE) cooling heating Eutectic Reaction • Solvus – (solid solubility line) BC, GH • Solidus – AB, FG, BEG (eutectic isotherm) • Liquidus – AEF • Maximum solubility: α = 8.0 wt% Ag, β = 8.8 wt %Cu • Invariant point (where 3 phases are in equilibrium) is at E; CE = 71.9 wt% Ag,TE = 779C (1434F). • An isothermal, reversible reaction between two (or more) solid phases during the heating of a system where a single liquid phase is produced.

26. c10f08 Pb-Sn Phase Diagram Liquidus Solidus Solidus Solidus Solvus Solvus

27. Solidification of Eutectic Mixtures • Mixtures of some metals, such as copper & nickel, are completely soluble in both liquid and solid states for all concentrations of both metals. Copper & nickel have the same crystal structure (FCC) and have nearly the same atomic radii. The solid formed by cooling can have any proportion of copper & nickel. Such completely miscible mixtures of metals are called isomorphous. • By contrast, a mixture of lead & tin that is eutectic is only partially soluble when in the solid state. Lead & tin have different crystal structures (FCC versus BCT) and lead atoms are much larger. No more than 18.3 weight % solid tin can dissolve in solid lead and no more than 2.2% of solid lead can dissolve in solid tin (according to previous phase diagram). • The solid lead-tin alloy consists of a mixture of two solid phases, one consisting of a maximum of 18.3 wt% tin (the alpha phase) and one consisting of a maximum of 2.2 wt% lead (the beta phase).

28. (Ex 1) Pb-Sn Eutectic System T(°C) 300 L (liquid) a L + a b b L + 200 183°C 18.3 61.9 97.8 C- C0 150 W  = C- C 100 a + b 99 - 40 59 = = = 0.67 99 - 11 88 100 0 11 20 60 80 99 40 C0- C W C C  C0 = C, wt% Sn C - C 40 - 11 29 = = 0.33 = 99 - 11 88 • For a 40 wt% Sn-60 wt% Pb alloy at 150°C, determine: -- the phases present Pb-Sn system Answer: a + b -- the phase compositions Answer: Ca = 11 wt% Sn Cb = 99 wt% Sn -- the relative amount of each phase Answer:

29. (Ex 2) Pb-Sn Eutectic System T(°C) CL - C0 46 - 40 = W = a CL - C 46 - 17 300 L (liquid) 6 a L + = = 0.21 29 220 a b L + 200 b 183°C 100 a + b 100 17 46 0 20 40 60 80 C CL C0 C, wt% Sn C0 - C 23 = WL = = 0.79 CL - C 29 • For a 40 wt% Sn-60 wt% Pb alloy at 220°C, determine: -- the phases present: Answer: a + L -- the phase compositions Answer: Ca = 17 wt% Sn CL = 46 wt% Sn -- the relative amount of each phase Answer:

30. Pb-Sn • For lead & tin the eutectic composition is 61.9 wt% tin and the eutectic temperature is 183ºC -- which makes this mixture useful as solder. • At 183ºC, compositions of greater than 61.9 wt% tin result in precipitation of a tin-rich solid in the liquid mixture, whereas compositions of less than 61.9 wt% tin result in precipitation of lead-rich solid.

31. Microstructural Developments in Eutectic Systems - I T(°C) L: C0 wt% Sn 400 L a L 300 L a + a 200 a: C0 wt% Sn TE 100 b + a 0 10 20 30 C , wt% Sn C0 2 (room T solubility limit) • For alloys where C0 < 2 wt% Sn • Result at room temperature is a polycrystalline with grains of a phase having composition C0 Pb-Sn system

32. Microstructural Developments in Eutectic Systems - II L: C0 wt% Sn T(°C) 400 L L 300 a L + a a: C0 wt% Sn a 200 TE a b 100 b + a 0 10 20 30 C , wt% Sn C0 2 (sol. limit at T ) 18.3 room (sol. limit at TE) Pb-Sn system 2 wt% Sn < C0 < 18.3 wt% Sn • Results in polycrystalline microstructure with agrains and small b-phase particles at lower temperatures.

33. cooling heating c10f13 Microstructures in Eutectic Systems - III • Co = CE • Results in a eutectic microstructure with alternating layers of aandbcrystals. Pb-Sn system

34. Lamellar Eutectic Structure • A 2-phase microstructure resulting from the solidification of a liquid having the eutectic composition where the phases exist as a lamellae that alternate with one another. • Formation of eutectic layered microstructure in the Pb-Sn system during solidification at the eutectic composition. Compositions of αandβphases are very different. Solidification involves redistribution of Pb and Sn atoms by atomic diffusion. Pb-rich Sn-rich

35. Pb-Sn Microstructures The dark layers are Pb-rich α phase, the light layers are the Sn-rich β phase.

36. Copper phosphorus eutectic Ni-Al Pb-Sn 20mol% CeO2-80mol% CoO. Ir-Si

37. Microstructures in Eutectic Systems - IV Pb-Sn system • Just above TE : L T(°C) L: C0 wt% Sn  Ca = 18.3 wt% Sn L  CL = 61.9 wt% Sn 300 L Wa  = 0.50 L + = a b WL = (1- W ) = 0.50  L + a 200 TE • Just below TE : C = 18.3 wt% Sn    100 + C  = 97.8 wt% Sn a eutectic b eutectic W  = 0.727 = 0 20 40 60 80 100 W = 0.273 wt% Sn  18.3 61.9 97.8 C, wt% Sn • For alloys with18.3 wt% Sn < C0 < 61.9 wt% Sn • Result:a phase particles and a eutectic microconstituent CL - C0 CL - C Primary α Cβ - C0 Cβ - C

38. Chapter 10 (part 2) • Equilibrium Diagrams with Intermediate Phases or Compounds • Eutectoid and Peritectic Reactions • Ceramic Phase Diagrams • The Gibbs Phase Rule • The Iron-Iron Carbide Phase Diagram • Development of Microstructures in Iron-Carbon Alloys • Hypoeutectoid Alloys • Hypereutectoid Alloys • Influence of Other Alloying Elements

39. Intermetallic Compounds 19 wt% Mg-81 wt% Pb Mg2Pb Note: intermetallic compounds exist as a line on the diagram - not a phase region. The composition of a compound has a distinct chemical formula.

40. c10f19 Cu-Zn System (Brass) Cartridge brass: 70 wt% Cu

41. Peritectic transformation  + L Eutectoid transformation  +  Eutectoid & Peritectic Cu-Zn Phase diagram

42. cool cool cool heat heat heat Eutectic, Eutectoid, & Peritectic • Eutectic - liquid transforms to two solid phases L  +  (For Pb-Sn, 183C, 61.9 wt% Sn) • Eutectoid – one solid phase transforms to two other solid phases • Solid1 ↔Solid2 + Solid3 •  + Fe3C (For Fe-C, 727C, 0.76 wt% C) • Peritectic - liquid and one solid phase transform to a 2nd solidphase • Solid1 + Liquid↔ Solid2 •  + L ε(For Cu-Zn, 598°C, 78.6 wt% Zn)

43. Ceramic Phase Diagrams MgO-Al2O3 diagram: 

44. APPLICATION: REFRACTORIES • Need a material to use in high temperature furnaces. • Consider Silica (SiO2) - Alumina (Al2O3) system. • Phase diagram shows: mullite, alumina and crystobalite(made up of SiO2) are candidate refractories.

45. Ceramic Phases and Cements

46. Gibbs Phase Rule • Phase diagrams and phase equilibria are subject to the laws of thermodynamics. • Gibbs phase rule is a criterion that determines how many phases can coexist within a system at equilibrium. P + F = C + N P: # of phases present F: degrees of freedom (temperature, pressure, composition) C: components or compounds N: noncompositional variables For the Cu-Ag system @ 1 atm for a single phase P: N=1 (temperature), C = 2 (Cu-Ag), P= 1 (a, b, L) F = 2 + 1 – 1= 2 This means that to characterize the alloy within a single phase field, 2 parameters must be given: temperature and composition. If 2 phases coexist, for example, a+L , b+L, a+b, then according to GPR, we have 1 degree of freedom: F = 2 + 1 – 2= 1. So, if we have Temp or composition, then we can completely define the system. If 3 phases exist (for a binary system), there are 0 degrees of freedom. This means the composition and Temp are fixed. This condition is met for a eutectic system by the eutectic isotherm.

47. Iron-Carbon System • Pure iron when heated experiences 2 changes in crystal structure before it melts. • At room temperature the stable form, ferrite (a iron) has a BCC crystal structure. • Ferrite experiences a polymorphic transformation to FCCaustenite (g iron) at 912 ˚C (1674 ˚F). • At 1394˚C (2541˚F) austenite reverts back to BCC phase d ferrite and melts at 1538 ˚C (2800 ˚F). • Iron carbide (cementite or Fe3C) an intermediate compound is formed at 6.7 wt% C. • Typically, all steels and cast irons have carbon contents less than 6.7 wt% C. • Carbon is an interstitial impurity in iron and forms a solid solution with the a, g, d phases.

48. c10f28 Iron-Carbon System